advertisement

FREQUENCY-DEPENDENCE OF RELATIVE PERMEABILITY IN STEEL N. Bowler Iowa State University, Center for Nondestructive Evaluation, Applied Sciences Complex II, 1915 Scholl Road, Ames, IA 50011, USA ABSTRACT. A study to characterize metal plates by means of a model-based, broadband, four-point potential drop measurement technique has shown that the relative permeability of alloy 1018 low-carbon steel is complex and a function of frequency. A magnetic relaxation is observed at approximately 5 kHz. The relaxation can be described in terms of a parametric (Cole-Cole) model. Factors which influence the frequency, amplitude and breadth of the relaxation, such as applied current amplitude, sample geometry and disorder (e.g. percent carbon content and surface condition), are considered. Keywords: permeability measurement, magnetic relaxation, 4-point ACPD, carbon steel PACS: 41.20.-q, 75.50.Bb INTRODUCTION A study to characterize metal plates by means of a model-based, broadband, four-point potential drop measurement technique [1] has shown that the relative permeability, µ, of an alloy 1018 carbon-steel plate is complex and a function of frequency: µ(ω) = µ0 (ω) + iµ00 (ω), (1) with ω = 2πf being angular frequency. For measurements made in the frequency range 1 Hz to 100 kHz, a clear relaxation in the relative permeability is observed at around 5 kHz, with the real part declining from a value of approximately µ0 = 280 at low frequencies (1 to 10 Hz), depending on the amplitude of the injected current, to approximately 90 at 100 kHz. Possible mechanisms responsible for this effect include phase lag in the motion of magnetic domain walls, with respect to the applied alternating current injected into the plate [2], or the presence of a surface region in which the material structure and its electromagnetic properties have been modified, compared with the bulk, for example by processing methods such as cold-rolling. The need for a complex, frequency-dependent magnetic permeability has also been recognized in studies on various ferromagnetic metal plates subjected to a homogenous time-harmonic magnetic field, with impedance measurements made by a pick-up coil wrapped around the specimen [3]. Here, the observed magnetic relaxation is characterized in terms of a parametric model [2]. Factors which influence the frequency, amplitude and breadth of the relaxation, such as sample geometry, amplitude of the applied current and disorder in the steel (e.g. percent carbon content and surface condition), are considered. CP820, Review of Quantitative Nondestructive Evaluation Vol. 25, ed. by D. O. Thompson and D. E. Chimenti © 2006 American Institute of Physics 0-7354-0312-0/06/$23.00 1269 air 6 conductive plate T p 0q −S ? 6 66 air l I 6 q 6 S 6 ¶³ ? V µ´ ¶³ I ? ∼ µ´ FIGURE 1: Four point probe in contact with a conductive plate. The probe points are arranged along a straight line. I is the amplitude of the applied alternating current. A proper understanding of the observed frequency-dependence of µ is important for correct interpretation of alternating-current potential drop (ACPD) measurements for the purpose of characterizing surface treatments such as case-hardened layers in steels. SPECIMEN The chemical composition of the alloy 1018 low-carbon steel plate is given in Table 1. The thickness of the plate was measured using digital calipers: T = 6.30 ± 0.01 mm. Other dimensions are 616 × 619 mm. It was not possible to anneal the specimen due to its large size. It was attempted to demagnetize the plate point-by-point using a C-core magnet on its surface, since it was too large to fit inside readily-available demagnetizing coils. This method may leave residual magnetization in local regions of the plate. FOUR-POINT ALTERNATING CURRENT POTENTIAL DROP EXPERIMENT A schematic diagram of a four-point probe in contact with a conductive plate is shown in Figure 1. Elsewhere it has been derived that, for this configuration, the voltage V measured between pick-up points at p and q can be expressed [1] " # " # I ik (S − p)(S + q) V = − coth(ikT ) + iωµ0 l ln , 2π σ (S + p)(S − q) T < 0.3S. (2) In equation (2), k = (1 + i)/δ where δ = (2/ωµ0 µσ)1/2 is the electromagnetic skin depth in the conductor, µ0 = 4π × 10−7 H/m is the permeability of free space, µ and σ are the relative magnetic permeability and conductivity of the plate, respectively, and I is the amplitude of the alternating current. Probe dimensions are shown in Figure 1. A series expansion analysis of equation (2) [1] permits derivation of the following expression, which describes a quasi-static regime in which the measured voltage is approximately real and constant, bounded by frequency fs whose value is chosen depending on the level of TABLE 1: Chemical composition (weight %) of alloy 1018 low-carbon steel. carbon manganese sulfur phosphorus iron 0.15 - 0.20 0.6 - 0.9 0.05 maximum 0.04 maximum remainder 1270 TABLE 2: Probe parameters. S (mm) 25.454 ± 0.005 p (mm) -10.152 ± 0.005 q (mm) 10.162 ± 0.005 l (mm) (fitted value) 0.15 ± 0.1 −5 1.06 x 10 experiment theory, σ = 5.18 MS/m 1.05 real voltage (V) 1.04 1.03 1.02 1.01 1 −2 10 −1 10 frequency (Hz) FIGURE 2: ACPD voltage measurements compared with theory in the quasi-static regime (f < 0.46 Hz). accuracy required. # " Vs = I (S − p)(S + q) ln , 2πσT (S + p)(S − q) For 0.1% accuracy in Vs , fs = 3 √ . 20 2πµσT 2 f < fs . (3) (4) From experimental results described later it will be seen that fs ≈ 0.46 Hz for this plate. Four sprung, point contacts were mounted in a plastic support block. The four points were arranged along a straight line, and the separation of the contacts was measured using a traveling microscope. With reference to Figure 1, the dimensions of the probe are listed in Table 2. Other details of the experimental arrangement have been described elsewhere [1]. DETERMINATION OF PLATE CONDUCTIVITY The conductivity of the plate was determined from comparison of ACPD voltage measurements in the quasi-static regime with theoretical expressions (3) and (4), Figure 2. Details of the procedure and analysis of uncertainties are given in reference [4]. The conductivity of the plate was determined to be 5.18 ± 0.04 MS/m. DETERMINATION OF PLATE PERMEABILITY With known conductivity, the permeability of the plate can be obtained by adjusting µ(ω) in equation (2) to achieve agreement between experimentally-measured and calculated voltage values. This was done on a point-by-point basis in the frequency range 1 Hz to 100 kHz to obtain the curves shown in Figure 3. A strong relaxation in µ(ω) is seen at approximately 5 kHz. The low-frequency limiting value of µ(ω) depends somewhat on the amplitude of the drive current. The drive current itself is real and constant over the majority of the measurement frequency range, but reduces in magnitude and undergoes a phase shift at higher frequencies, as shown in Figure 4. 1271 60 imaginary relative permeability 300 real relative permeability 250 200 150 100 50 1 10 initial current 2.47 A 1.23 A 0.61 A 0.31 A 2 10 3 10 frequency (Hz) 50 40 30 20 10 4 10 0 1 10 5 10 2 10 3 10 frequency (Hz) 4 10 5 10 FIGURE 3: Real and imaginary parts of complex permeability as a function of frequency. 4 2.5 3 current phase (rad) current magnitude (A) 2 1.5 1 2 1 0 −1 0.5 −2 0 1 10 2 10 3 10 frequency (Hz) 4 10 5 10 −3 1 10 2 10 3 10 frequency (Hz) FIGURE 4: Magnitude and phase of driving current as a function of frequency. 1272 4 10 5 10 1 0.5 0.9 0.45 real relative permeability 0.7 imaginary relative permeability ν = 0.0 0.2 0.4 0.6 0.8 0.6 0.5 0.4 0.3 0.2 0.1 0 0 10 0.4 0.35 0.3 0.25 0.2 0.15 0.1 0.05 2 4 10 10 6 10 0 0 10 2 4 10 frequency (Hz) 10 6 10 frequency (Hz) FIGURE 5: Real and imaginary parts of relative permeability as a function of frequency, calculated using equation (5), for various values of the parameter ν. The relaxation time t is chosen arbitrarily to be 1 kHz. Similarly, µ0 (0) = 1 and µ0∞ = 0. TABLE 3: Low-frequency, real permeability, µ0 (0). initial current (A) µ0 (0) 2.47 285 ± 2 1.23 269 ± 2 0.61 259 ± 2 0.31 251 ± 2 PERMEABILITY MODEL For a constant amplitude of applied magnetic field, the complex permeability may be written [2] µ0 (0) − µ0∞ + µ0∞ , µ(ω) = (5) 1 − iωτ (ω) in which µ0 (0) and µ0∞ are the low- and high-frequency, constant, real relative permeability values for the relaxation process, respectively, and τ (ω) represents a relaxation ‘time’ that may be complex. Equation (5) reduces to the Debye form of relaxation if τ (ω) = t = constant. The Cole-Cole representation is obtained for τ (ω) = ω −ν t1−ν eiνπ/2 , ν ≥ 0. (6) The Debye form is recovered from (6) when ν = 0. In Figure 5, µ is plotted for various values of the parameter ν. It can be seen that increasing ν gives broader relaxation while reducing the magnitude of the loss peak in the imaginary permeability. In Figure 6, parametric curves are compared with experimental data. Calculated curves shown in Figure 6 are obtained with parameters µ0∞ = 78, 1/t = 5 kHz and ν = 0.4. The same data are displayed in a permeabilityplane plot in Figure 7. For each value of initial applied current, µ0 (0) is obtained by taking the mean of the first few low-frequency data points. The values obtained are listed in Table 3 and plotted as a function of initial applied current in Figure 8. DISCUSSION The experimental data for µ0 is reproduced very well by the theoretical curves except in the highest frequency decade (104 to 105 Hz). The magnitude of the peaks in µ00 is also well-reproduced by theory, whereas the experimental data exhibits some asymmetry. These 1273 60 imaginary relative permeability 300 real relative permeability 250 200 150 100 50 1 10 initial current 2.47 A 1.23 A 0.61 A 0.31 A model 2 10 50 40 30 20 10 3 4 10 frequency (Hz) 10 5 10 0 1 10 2 10 3 10 frequency (Hz) 4 10 5 10 FIGURE 6: Experimental and modelled real and imaginary parts of relative permeability as a function of frequency. Modelled values are calculated using equations (5) and (6), with parameters µ0∞ = 78, 1/t = 5 kHz and ν = 0.4. µ0 (0) for each value of initial applied current is listed in Table 3. imaginary relative permeability 60 50 40 30 20 initial current 2.47 A 1.23 A 0.61 A 0.31 A model 10 0 50 100 150 200 real relative permeability 250 300 FIGURE 7: Permeability-plane plot of experimental and modelled complex permeability. 285 280 µ′(0) 275 270 265 260 255 250 0 0.5 1 1.5 initial current (A) 2 2.5 FIGURE 8: Low-frequency, real permeability, µ0 (0), as a function of initial applied current amplitude. 1274 25 100 real relative permeability 90 imaginary relative permeability iron quenched steel 80 70 60 50 40 20 15 10 5 30 20 0 10 1 2 10 10 3 10 0 0 10 1 2 10 10 3 10 frequency (Hz) frequency (Hz) FIGURE 9: Real and imaginary parts of complex permeability as a function of frequency for measurements on iron and quenched steel. Data is taken from reference [3]. discrepancies may be attributed to the significantly reduced amplitude of the drive-current in the frequency range 104 to 105 Hz, as shown in Figure 4, since the model assumes constant amplitude of the applied magnetic field, H, whereas H is proportional to I. In addition, injecting current by means of a four-point probe clearly gives rise to a spatially-varying magnetic field whose amplitude at any one field point depends on the geometry of the specimen and the probe. It is also possible that microstructural changes near the surface of the specimen, for example due to cold-finishing, may give rise to changes in the electromagnetic properties of the steel in a surface region. This means that µ may also vary as a function of depth in the specimen, in a way not represented by equations (5) and (6). It is not surprising that the observed relaxation is broader (with ν = 0.4) than a Debye relaxation (ν = 1) since most physical systems exhibit microstructural inhomogeneities which give rise to a distribution of relaxation times, here embedded in the function τ (ω). The variation of µ0 (0) as a function of the amplitude of the initial current, Table 3 and Figure 8, is explained by the fact that the magnetic field, H, in the specimen is proportional to the applied current. As the applied current changes, H also changes and a different point on the magnetization curve for the material (the curve of B versus H) is reached. The value of µ0 (0) changes according to the slope of the magnetization curve. CONCLUSION Magnetic relaxation has been observed in measurements made on an alloy 1018 carbonsteel plate by a model-based four-point alternating-current potential drop technique. A possible mechanism responsible for this phenomenon is phase lag of domain wall motion, either bowing or movement between pinning sites, with respect to the applied field. The phenomenon may therefore be expected to be disorder-dependent, related to the density of pinning sites in the material, which in turn may be related to the percent carbon content in steel, for example. Indeed, relaxation in µ has not been observed in similar experiments on spring steel [1] and an independent study has shown a difference in behavior between iron and quenched steel [3], as shown in Figures 9 and 10. Surface condition and processing history of the sample may also play a role, since both of these influence the density and nature of domain-wall pinning sites. The phenomenon at work here may be responsible for the inability to fit eddy-current impedance data, taken on iron and high-purity nickel samples, using standard models assuming homogeneous material properties [5]. Further work is necessary to identify precisely the mechanism(s) responsible for the observed frequency-dependence of µ. 1275 imaginary relative permeability 25 20 15 10 iron quenched steel 5 0 20 40 60 80 real relative permeability 100 FIGURE 10: Permeability-plane plot of data shown in Figure 9. ACKNOWLEDGMENTS This work was supported by the NSF Industry/University Cooperative Research program. The author thanks Y. Huang for assistance with processing the data presented in Figure 3. REFERENCES 1. N. Bowler and Y. Huang, IEEE Trans. Mag. 41, 2102–2110 (2005). 2. J. Sláma, P. Krivošı́k and V. Jančárik, J. Magnetism and Magnetic Materials 215–216, 641–643 (2000). 3. V. A. Sandovskii, V. V. Dyakin and M. S. Dudarev, Russian J. Nondestr. Testing 33, 52–55 (1997). 4. N. Bowler and Y. Huang, Meas. Sci. Tech., accepted August 2005. 5. J. C. Moulder, C.-C. Tai, B. F. Larson and J. H. Rose, IEEE Trans. Mag. 34, 505–514 (1998). 1276